Physiochemical properties of clay nanoparticles .
Clay nanoparticles are among the most applicable and cost-affordable materials, all of which have a variety of applications in case of medical science. In this chapter, key characteristics of the clay nanoparticles along with their major groups, structure, morphology, and physicochemical properties were evaluated. Thereafter, the applications of clay nanoparticles in the field of nanocomposite, polymeric matrices, and medicine were investigated, while specimen production procedures were also reviewed. The main focus of this chapter is to investigate the applications of clay nanoparticles in bio- and medical science. In fact, organically modified clay nanoparticles (organoclays) are an attractive class of hybrid organic–inorganic nanomaterials with potential applications in case of polymer nanocomposites, rheological properties modification, and drug delivery carrier.
- clay nanoparticle
Clay nanoparticles are natural materials in nanoscale that originate from clay. They have attracted much attention in recent years due to their widespread applications. The interest in exploiting clay nanoparticles for various purposes is due to their high surface and unique physical and chemical properties.
In 2013, a group of researchers focused on clay nanoparticles as a drug delivery system. Preparation, physical/chemical properties, and bioaccumulation of clay nanoparticles based on drug delivery systems, as well as their application in the food system as a nanocarrier for vitamins, antioxidants, linoleic acid, and the other foods, were discussed . In addition, studies have shown that nanotechnology will revolutionize the food industry . Nanoscale food control can lead to the correction of micromolecular properties of foods such as taste, aroma, texture, sensory characteristics, processing ability and stability throughout the process, and storage. Nanotechnology applications grow rapidly in the food and ingredient sector. Advanced nanoelectronics, in combination with good nanomaterials and intelligent biological components, are able to develop very specific and selective measuring devices to identify potentially hazardous agents, including viruses, pathogenic microorganisms, as well as inappropriate physical and chemical substances in foods [3–5]. The micro/nanotechnology accelerates the decreasing size of the sensor to the extent appropriate for application (applied field) [6–8].
In addition to ensuring food safety, nanotechnology improves our lives by monitoring quality and nutrition status [9, 10]. Food packaging is another area that has used nanomaterials to increase the shelf life of the food by improving the preserving properties. Nylon-based nanocomposites are currently used to produce beverage bottles in Korea and the United States . Polymer nanoparticles are made by dispersing nanoparticles into a polymer matrix . For example, nylon/silicate nanocomposite containing 2% non-mineral nanoparticle has two times higher tensile strength and thermal stability (at a temperature above 100°C) than pure nylon . Nylon-based nanocomposites are formed by the dispersion of silicate layers on a continuous polymer matrix. This structure significantly reduces the amount of oxygen or carbon dioxide release (diffusion) in encapsulation, since these gases should be distributed through the space between dispersed nano-silicate layers . Properties such as strength and thermal stability make this nanocomposite ideal for packaging food. Several attempts and experiments have been carried out to provide various types of antioxidants, nutrients, minerals, drugs, and other applicable factors through food . Currently, most efforts to develop delivery systems focus on drugs. While safety and cost concerns are one of the most important factors in choosing food for the customer, high production costs of drug delivery systems are still acceptable in medicine. Clay nanoparticles are minerals in clay that have attracted much attention due to the biological application of their abundance in nature, simplicity of construction, and biocompatibility [15–18]. Clay nanoparticles also have a great potential for nutrition because they have been used to treat and protect as a traditional medicine since the beginning of human civilization [19–21]. Clay minerals have been used as laxatives, antidiarrhea, anti-inflammatory agents, blood purification, reducing infections, and healing of stomach ulcers . In addition, biocompatible clay minerals are currently used as oral antioxidants [23, 24]. Clay nanoparticles have unique layer structures, including the accumulation of nanoparticles with metal ions and intracellular ions for charge balancing . The two-dimensional (2D) structure illustrates interesting strategies for the development of new nano-hybrid systems by enhancing active biochemical molecules into space (Figure 1). Intrinsically, unstable agents can be protected against processing conditions and hard-working environment and ultimately released with a controlled pattern in a desirable environment [26–28]. Many studies have shown that nano-layered materials can encapsulate DNA [29, 30], nucleotides [31, 32], drugs [33, 34], proteins , and even viruses . These nano-hybrid systems are designed to enhance the efficient delivery to cells and the effectiveness of biochemical molecules [37–39]. However, the application of nanoscale materials to nutrients delivery is very limited.
2. Delivery efficiency and biocompatibility of clay nanoparticles
2.1. Structural and physical properties of nanoclays
Nanoclays are fine-grained crystalline materials. A layer is the basic structural unit of nanoclays, and these layers are prone to arrange themselves over one another like pages of a book. Individual layers are composed of the tetrahedral and/or octahedral sheets, and this arrangement of sheets plays a vital role in defining and distinguishing these clay minerals. In tetrahedral sheet, the silicon-oxygen tetrahedra are linked to neighboring tetrahedra by sharing three corners while the fourth corner of each tetrahedron forms a part to the adjacent octahedral sheet. The octahedral sheet is usually composed of aluminum or magnesium in a sixfold coordination with oxygen from the tetrahedral sheet and with hydroxyl.
2.2. Structural features
Clay layer nanoparticles are divided into two different types of anion and cation depending on the level of layer charge and the types of interlayer ions. Anionic layer nanomaterials typically have been created by double-layered hydroxides (LDHs) with alterable anions in interlayer spaces. LDHs include a wide range of chemical compounds and their layered structure that can be of a great variety to produce poly-types. For example, aluminosilicate cationic nanoparticles like montmorillonite (MMT) have octagonal and quadrilateral plates with high internal surfaces. The main structure of cationic clays is based on a framework, where the unit structure is composed of an octagonal-twisted sheet between two quadrilateral plates. In Figure 2, the structure of the double-layer hydroxide and cationic clay (MMT) is presented.
Therefore, cationic and anionic clay nanoparticles can be applied as transfer carriers, which depend on the charge of molecules and essentially on their unique layered structure.
In general, clay nanoparticles are considered as biodegradable materials. In fact, cationic minerals have traditionally been applied in a variety of fields including skin chemotherapy, laxatives, antidiarrhea, and anti-inflammatory agents as well as antimicrobial agents [40–42]. Recently, they are used as lubricants and distributary in pharmaceutical programs to improve chemical, physical, and organoleptic properties [43–45]. MMT can be considered as an eco-friendly cationic clay , which is commonly used in many pharmaceutical formulations as an active and additive substance . In addition, anionic nanoparticles of LDH in carbonate form are used as an antacid agent (antipepsin) to neutralize gastric acid, which is related to its alkaline properties under physiological pH . The results show that LDH has a lower toxicity compared to single-walled carbon nanotubes and iron oxide and silica nanoparticles.
2.4. Clay nanoparticles for nutrient delivery systems
As previously described, clay nanoparticles are biocompatible materials with a high internal space, a high ion exchange capacity, and a low toxicity that these properties make them ideal for the bioactive compound delivery systems. The nanoclay encapsulation system can be prepared in a relatively simple and inexpensive process compared to other delivery systems. In addition to improving the solubility of the drug or active compounds, the nanoparticle encapsulation system has been considered for oral applications due to its high adhesion properties that are useful for molecules against GI barriers . Choi’s research team reports an easy way of encapsulating the strongest antioxidant by MMT with cation exchange reaction (Figure 3(A)) . γ-L-glutamyl-L-cysteinylglycine (GSH) is a cellular antioxidant protector (preserver) against reactive oxygen species by neutralizing free radicals. GSH stability can be increased by encapsulating GHS on MMT. The tested GSH-MMT on mice resulted in a significant increase in the bioavailability and high activity of antioxidants in the plasma (Figure 3(B)).
Clay nanoparticles have attracted a great deal of attention as a good candidate for packaging of various materials, and it clearly demonstrates the increase in the sustainability and bioavailability of functional molecules.
2.5. The effect of clay mineral nanoparticles on the growth performance of internal organs and blood biochemistry of chickens compared to vaccines and antibiotics
Al-Beitawi et al.  investigated the effect of three levels of nanoclay minerals (1, 1.5, and 2%) on the growth performance of internal organs and blood biochemistry of chickens compared to vaccines and antibiotics. The experiment was conducted in nine diets for more than 36 days . Groups 1–3 were fed with diet without clay mineral nanoparticles, and group C1 (positive with vaccines and antibiotics), C2 (positive only with vaccine), and C3 negative and without any of them (as control group). Treating groups with a similar diet to the levels mentioned earlier were done once or twice in a week. Performance of chickens, which fed with 2% clay nanoparticles, significantly improved in terms of body weight and feed conversion rates compared to control groups. With regard to blood biochemistry, high-density lipoprotein that is beneficial to the body was increased. Current results indicate that the mineral clay nanoparticles at certain levels and doses improve the performance of chickens. Nanotechnology is considered as a new potential tool for improving broiler chickens. Researchers believe that the beneficial and positive effects of the use of mineral clay nanoparticles as an additive to the diet of broiler chicks may be due to several factors such as the concentration, dose, and nature of nanoparticles . Desai et al. observed that a nano-supplement form would increase the surface area, which may also increase the absorption and consequently the use of minerals . In addition, Weiss et al. reported that the size of nanoparticles may increase the function or bioavailability of nutrients and compounds . Mushtaq et al. reported that Na+ is the main cation of extracellular fluids involved in several functions including acid-base balance and amino acid absorption and glucose utilization that is beneficial for body growth, which may have a significant improvement in the growth performance of broiler chickens. On the other hand, the interest in using nanotechnology as a new tool in feeding broiler chicks shows that nanoparticles have very different physical and chemical properties from large particles . In 2013, Sawors et al. suggested that the number of muscle cells returns to genetic, environmental, and nutritional factors . On the other hand, creating more accessible mineral resources, such as clay nanoparticles, can have positive effects on tissue development. According to the obtained results, it can be concluded that the mineral clay nanoparticles have a favorable effect on total serum protein and its cleft . Nanoparticles have been reported to exhibit several new characteristics of transfer and absorption and also have more effective absorption. The researchers suggested that the superior performance of clay nanoparticles may be due to smaller size and larger surfaces that improve intestinal absorption .
2.6. Evaluation of the clay nanoparticles toxicity in epithelial cells
The extending continuous use of products containing nanoparticle for a wide range of applications has raised public health and safety concerns. Although products containing clay nanoparticles cannot be toxic, human contact during its preparation, production, or disposal process can have undesirable effects on health, which makes it necessary to evaluate the biocompatibility of clay nanoparticles. A group of researchers examined the effects of platelet toxicity (Bentone MA, ME-100, Cloisite Na+, Nanomer PGV, and Delite LVF) on human lung . They used automated cells for the first time in real-time impedance imaging compositions and also showed the effect of toxicity on the difference in the dose level and the time-dependent of both types of clay nanoparticles . Clay nanoparticles are used in a wide range of modern products such as electronic, food, clothing, tire, medicine, sunscreen, cosmetics, sports equipment, polymer composites, bone implantation, controlled drug delivery systems, protective coatings (such as anti-corrosion, antibacterial, or antimolding), and for the synthesis of materials . Clay nanoparticles, for example, plastic nanocomposites, are being developed to create unique devices for the next generation of biological applications, including antimicrobial agents, drug delivery, and cancer treatment [59–62].
2.7. Characterization of clay nanoparticles
SEM and TEM images are shown in Figure 4. In Table 1, a summary of the physiochemical properties of clay nanoparticles such as purity, specific surface area, zeta potential, and so on has been shown, which essentially affects the absorption and toxicity of nanoparticles.
|Geometry||Nanoclay||Chemical formula||Purity (%)||Zeta potential (Mv)||Specific surface area (m2/g)|
|Tubular||Halloysite MP1||Al2Si2O5(OH)4 × 2H2O||90||−41||65|
|Halloysite||Al2Si2O5(OH)4 × 2H2O||90||−32.1||64|
|Platelet||Nanomer PGV||M+y(Al2-yMgy)(Si4)O10(OH)2 × nH2O||100||−51.9||ND|
2.8. Application of nanoclay-based composites in bone tissue engineering
The properties of MMT clay, such as its ability to absorb various types of toxins and the ability to cross the digestive tract (stomach and intestines) [60, 63–66], along with the ability to carry and transfer the drug [67–71], encourage human to use it in tissue engineering applications. It is reported that these nanoparticles are removed from the body because they cannot be absorbed by the intestines and they can also be dissolved by the acids in the stomach or intestine . In addition, clay is used as an edible laxative and an antidiabetes . The above suggests that clay is suitable for tissue engineering applications, and decomposed products can be disposed without any effects on the normal body function. The use of MMT clay for bone tissue engineering applications needs further research. In the few studies that have been done in the past, MMT has been used to prepare nano-composites that examine the effect of adding clay on the mechanical and biological properties of polymers [73, 74]. Researchers have used 5-aminovaleric acid-modified MMT clay to prepare polymer composites for bone tissue engineering studies .
2.9. Montmorillonite (MMT) as a carrier for drug delivery
Clay as a carrier for drug delivery is an amazing interdisciplinary field that brings together biology, materials science, and nanotechnology. Composites based on clay minerals have effect on a variety of fields, especially in pharmaceutical science. The tremendous variety of these natural materials has made the widespread collection of clays and polymers available to researchers [76–84]. The controlled drug delivery system is a method for the development of nanostructures and materials that can encapsulate high concentrations of materials, pass through a cell membrane, and release the drug in the target region for a given period. Clay minerals have exceptional (unique) characteristics such as low toxicity, better biocompatibility, and are guaranteed for a controlled drug release, and thus they are used in biological applications in pharmaceuticals, cosmetics, and even medical purposes [85, 86]. MMT is a natural mineral clay with a layered structure and prominent features such as a high internal surface area and cation exchange capacity (CEC), a high absorption capacity, and low toxicity [64, 87]. MMT with a net charge of the network can well be swollen in the presence of water and hydrophilic solvents, because positive-charged bioactive compounds can be inserted in interlayer (inside layer) spaces by electrostatic interaction. Many attempts have been made to develop MMT as a carrier for drug delivery, for example, to improve the water solubility of insoluble drugs and control the release of bioactive molecules [61, 83, 84, 88–93]. Biochemical properties, which make clay valuable for pharmaceutical applications, include high absorption capacity, high internal surface, high exchange ability, interlayer spatial reactions with drug molecules, chemical moisture, and low toxicity [61, 72, 83, 84, 94–96]. Clay is widely used as an active agent and an additive in pharmaceutical formulations [97–99]. In pharmaceuticals, MMT has found extensive applications as a suspension and a stabilizer, as well as an absorbent and clear factor. Also, MMT has been used as a drug carrier or an additive in pharmaceutical formulations [71, 72, 99–104]. The MMT’s ion exchange capacity provides the possibility of replacing Na + with other organic and inorganic cations to increase performance. It also causes the use of MMT and other clay species as a tissue regeneration agent [71, 76–84, 96, 105] (Table 2).
|5-Flurouracil (anticancer)||Ibuprofen (nonsteroidal anti-inflammatory)|
|Amino acids||BSA (model protein)|
|Plasmid DNA (gene delivery)||Donepezil (Alzheimer)|
|Paclitaxel (anticancer drug)||Docetaxel (anticancer drug)|
|Lidocaine (local anesthetic drug)||5-Fluorouracil (anticancer drug)|
|Glutathione (antioxidant)||Doxorubicin (anticancer drug)|
|Ibuprofen (anti-inflammatory)||Buspirone hydrochloride (antianxiety)|
|Captopril (hypertension)||Timolol maleate (β-adrenergic blocking agent)|
|Vitamin B1||Ranitidine hydrochloride (antacid)|
|Quinine (antimalarial drug)||Procainamide hydrochloride (antiarrhythmia drug)|
|Tamoxifen (anticancer drug)||Epidermal growth factor (tissue engineering)|
The authors have shown that increasing the concentration of silicate nanoparticles increases the mechanical strength of polymer nanoparticles . Wang et al. prepared 2008 complex chitosan-montmorillonite (HTCC/MMT) nanocomposites for the application as protein carriers . In 2010, Shhameli et al. showed a new green color combination for MMT/chitosan nanoparticles (CS) and its antibacterial actions . Lee and Fu found that the properties of the released drug can be controlled by the charge of N-isopropylacrylamide/MMT nanocomposites . In general, the ability to exchange ions, interoperability, and biocompatibility of MMT has made it an ideal candidate for drug delivery. In addition to pharmaceutical use, MMT and its nanocomposites are bioactive agents that have a wide range of applications. MMT can play an important and powerful role in intestinal detoxification, since it can absorb food, microbial, and metabolic toxins and, surprisingly, can increase the hydrogen ions in acidosis. Also, MMT can be used for edible purpose for digestive system detoxification, constipation reduction, internal parasite eradication, strengthening of the immune system, liver detoxification, reduction of stomach pain, and poisoning by bacteria. Revitalizing drugs and tissue engineering programs include bone remodeling as growth agents and wound dressing. The network structure of this is shown in Figure 5 .
MMT is widely used in the treatment of bone pain and damaged muscle, chronic headache, open wounds, special skin conditions (acne, eczema, red seeds on the skin, etc.), diarrhea, hemorrhoids, stomach ulcers, intestinal problems, anemia, rapid recovery of injuries (bruises, stretching, burns, etc.), severe bacterial infections, skin rejuvenation, and various health issues. Therefore, it can be beneficial to health because all its activities are physical and there is no chemical reaction on the body. After taking, no or small amount of MMT is absorbed in the digestive system and the rest is excreted (repulsed) by feces. According to the ISI database, interest in drug delivery by clay shows a significant increase in scientific publications (Figure 6) .
2.10. Mechanisms of drug-clay interactions
According to the tests conducted, the basis of controlled drug delivery is the use of laminar (layer) interference. Interference may occur by mixing sub-solids (ion converters) with ionic material in solution. In biological fluids, “anti-ions” can move the drug into the substrate and transfer it to the body, so the converter can be removed or decomposed at the end (Figure 7) . Smectites, especially MMT and saponite, have been further studied due to their ionic exchange capacity compared to other silicates (talc, kaolin, and fibrous mineral clay). A specific mechanism depends on factors such as functional groups and chemical physical properties of organic compounds [109–111]. Silicate-based composites exhibit a good inhibitory (barrier) effect due to complicated intrusive pathways that small molecules need to undergo (pass) in order to clarify the material (Figure 8) .
2.11. The latest MMT pattern used in drug delivery systems
Lin et al. showed the 5-FU interference on the MMT inner layers . 5-FU-MMT was determined and the successful interference of the drug in MMT was confirmed by opening the inner layer and changing the XRD pattern to the lower 2θ angle, and the results are presented in Figure 9. Finally, it can be concluded that the total amount of 5-FU absorbed in MMT is approximately 87.5 mg/g MMT.
Park et al. reported the placement of donepezil molecules on clay (Laponite, LA, saponite, SA and MMT) and provided descriptive information, which confirmed the well-located donepezil molecules in the inner layers of clay (Figure 10) . The absorption amount and the donepezil molecular structure depend on the cationic exchange ability of clay, which has designed drug release patterns. The rate of release can be increased easily by using a large cationic polymer. The Eudragit® E-100 hybrid, coated with such a polymer, shows the release of drug at higher speeds over a short period. Therefore, nanoclay materials are proposed as an advanced carrier for drug delivery with a controllable release feature.
2.12. 2D clay nanoparticles for drug delivery in cancer treatment
Two-dimensional kaolinite clay nanoparticles are used in the drug delivery system. The increasing of spacing of the kaolinite nanoparticles from 0.72 to 4.16 nm is due to the interference of guest species with different chain lengths of organic materials that can increase the drug delivery efficiency and reduce the toxicity of doxorubicin (DOX). The kaolinite (Kaolin) and kaolin compounds show a high level of biocompatibility and low toxicity against pancreatic cancer cells, gastric cancer, prostate cancer, breast cancer, esophageal cancer, and thyroid cancer diagnosis. However, lung cancer and leukemia require structural harder compounds for drug delivery. DOX-Kaolin and its internal contents exhibit more drug release rates in acidic environment than in the neutral environment. The use of two-dimensional clay nanoparticles for a drug delivery system can pave the way for high-performance nano-therapies with superior antitumor efficacy and significant reduction of side effects. As shown in Figure 11, it is used for the treatment of tumors .
2.13. An overview of clay chemistry
Broadly, clay minerals are structured of two principal units: tetrahedral (T) and octahedral (O) sheets [114, 115]. Each tetrahedron consists of a central cation (mostly Si4+) coordinated to four anions and linked to adjacent tetrahedra through three shared oxygens on the corners (basal oxygens Ob) forming an infinite 2D hexagonal mesh (Figure 12). The fourth (apical oxygen Oa) remains unshared, lying perpendicular to the tetrahedral sheet, and is the main site of interaction with the octahedral sheet. Each octahedron consists of a metal cation ( ) coordinated to six and/or anions. Adjacent octahedra are linked to each other by sharing edges (two or ), forming an octahedral sheet. If Mn is divalent ( ), a trioctahedral or a brucite-like sheet is produced, if it is trivalent ( ), then two out of every three octahedral sites are occupied, leaving a vacant site and the generation of a dioctahedral or a gibbsite-like sheet. Clays can be classified into 1:1 and 2:1 types according to the layering of T and O sheets. 1:1 (or T-O) clay minerals consist of a single T sheet linked to a single O sheet, and 2:1 (or T-O-T) clay minerals consist of a single O sheet sandwiched between two T sheets (Figure 12, Table 3).
|Family group||Species||Chemical formula||Charge/formula unit||CEC||Particle size (nm)|
|1:1||Serpentine-kaolin||Halloysite||Al2Si2O5(OH)4.nH2O||~0 ||~10 meq/100 g [121, 122]||Nanotube diameter of ~50 nm, lumen of ~15 nm, and length of ~1 mm [119, 126]|
|2:1||Smectites||Montmorillonite||Nam(Al2-mMgm)Si4O10(OH)2.nH2O||~0.2–0.6 ||~80–150 meq/100 g [121, 122]||~80–300 nm diameter and ~ 1 nm thickness [127, 129]|
|Laponite (synthetic hectorite)||Nah(Mg3-hLih)Si4O10(OH)2.nH2O||~25–30 nm diameter and ~ 1 nm thickness [120, 123]|
|Sepiolite-palygorskite||Sepiolite||X*(Mg, Al, Fe3þ)4(Si,Al)6O15(OH)2.nH2O||—||~4–40 meq/100 g [124, 125]||Nanofiber diameter of ~15 nm and length of ~200–400 nm [124, 128]|
In the case of smectites, an octahedral sheet of metal oxides (usually or ) is sandwiched between two tetrahedral silica sheets. Two types of charges originate on the smectite clay particle: (1) permanent negative charges on the surface due to isomorphous cation substitution in the tetrahedral and/or octahedral sheets (e.g., for Mg2+ in Laponite) balanced by exchangeable cations such as Na or in the interlayer gallery. (2) Positive (amphoteric) charges on the edges due to broken Si-O, Al-OH, and Mg-OH groups. At pH < Zero Point of Charge (ZPC), these edge charges become positive with anion exchange capacity, while at pH > ZPC, they become negative with a cation exchange capacity. Adapted with permission . Copyright 2014, John Wiley and Sons.
We focused on the investigation of the potential toxic effects caused by nanoclay particles currently used in tons in several industrial applications. Bentonite, montmorillonite, and kaolin are platy clay particles ranging from nanometers to micrometers, whereas halloysite nanotubes are hollow rod-like particles having a lumen diameter of ∼20 nm and a tube length ranging from 300 nm to 2 μm. Spherical silica nanoparticles were also used as a material mimicking the outer silica layer of the clays. Graphene oxide nanosheets having the shape and size close to smectite clays were selected as a material with a relatively high reported toxicity, 30, which was also confirmed in our study. The typical AFM images demonstrating the geometry and sizes of nanoparticles used in this study are given in Figure 13.
The nanoparticles used were suspended in water and added to protozoan media at a range of concentrations. Prior to toxicity investigation, the hydrodynamic diameters and surface potential of nanoparticles were determined using dynamic light scattering (DLS) and electrophoretic mobility measurements in water (Table 4) .
|Particles||Hydrodynamic diameter, nm||Zeta-potential, mV||AFM measured dimensions|
|Halloysite||510 ± 12||−25 ± 3||50 nm diameter, 400–1500 nm length|
|Kaolin||930 ± 22||−36 ± 1||300–700 nm width, 30–100 nm thick|
|Montmorillonite||1600 ± 60||−29 ± 1||300–600 nm width, 10–50 nm thick|
|Bentonite||3040 ± 660||44 ± 2||∼4 μm width, ∼100 nm thick|
|Silica||122 ± 3||−39 ± 6||120 nm diameter|
|Graphene oxide||1940 ± 90||−47 ± 2||2000 nm width, 2–10 nm thick|
2.15. Ecotoxicological profile
No ecotoxicological studies of nanoclay have been identified as of November 30, 2010. Since clay is a naturally occurring material for which environmental organisms have adapted throughout evolution, the inherent toxicity is expected to be low; however, issues related to small particle sizes may occur .
2.16. Toxicological profile
Today, few studies are available, and there is limited knowledge about the toxicity of nanoclays and the chemical derivatives that may be generated during the production and processing of polymer nanoclay composites. However, in general, nanoclay is not considered to pose a major health risk although a possible content of crystalline quartz may constitute a risk. Furthermore, functionalized nanoclays containing quaternary ammonium or phosphonium functional groups on the surface are described as potentially problematic, as ammonium and phosphonium ions in their pure form can cause asthma symptoms (NFA, 2010) .
Clay nanoparticles have traditionally been used in many applications such as treatment, skin chemotherapy, and medicine to improve the human health and life. In addition, they have recently been developed as additives, lubricants, and active materials in pharmaceutical formulation. Although their application in food science is relatively limited, they have the potential to deliver nutrients. Their unique structure is able to place bioactive molecules in the interior space. Nanoparticles that contain nutrients have the ability to protect GI against the environment and control the release features. They can enter the cell and with their adhesion properties facilitate the transfer of GI molecules against barriers. Also, they exhibit low toxicity. Research on the development of clay nanoparticles based on oral delivery systems for nutrients or functional compounds indicates that they are effective in protecting and controlling deliveries and also contributing to the increased bioavailability. The promising potential of the clay nanoparticles makes a new perspectives for the development of nano-based oral delivery systems. The toxicity of nanomaterials is a very important issue. In general, the results show that higher doses of clay nanoparticles result in the death of cells, which is a concern for medical applications. As an important point in the application of clay nanoparticles in delivery systems, to achieve clay-based controlled delivery systems, one of the best ways is to place organic molecules on the underlying layers of mineral clay. Besides, its composites can be used to improve properties.
Choi SJ, Kim YR. Bioinspired Layered Nanoclays for Nutraceutical Delivery System. In ACS Symp. Series. 2013. pp. 207-220
Egger S, Lehmann RP, Height MJ, Loessner MJ, Schuppler M. Antimicrobial properties of a novel silver-silica nanocomposite material. Applied and Environmental Microbiology. 2009; 75(9):2973-2976
Lim MC, Shin YJ, Jeon TJ, Kim HY, Kim YR. Analytical and Bioanalytical Chemistry. 2011; 400:777-785
Joung CK, Kim HN, Im HC, Kim HY, Oh MH, Kim Y. Sensors and Actuators B: Chemical. 2012; 161:824-831
Huang Y, Dong X, Liu Y, Li LJ, Chen PJ. Materials Chemistry. 2011; 21:12358-12362
Batt CA. Science. 2007; 316:1579-1580
Min J, Kim JH, Lee YS, Namkoong K, Im HC, Kim HN, Kim YH, Huh N, Kim YR. Lab on a Chip. 2011; 11:259-265
Yager P, Edwards T, Fu E, Helton K, Nelson K, Tam MR, Weigl BH. Nature. 2006; 442:412-418
Arora, Amit, Padua GW. Nanocomposites in food packaging. Journal of Food Science. 2010; 75(1):R43-R49
Malathi AN, Santhosh KS, Nidoni U. Recent trends of biodegradable polymer: biodegradable films for food packaging and application of nanotechnology in biodegradable food packaging. Current Trends in Technology and Science. 2014; 3(2):73-79
Blasco C, Pico Y. Trends in Analytical Chemistry. 2011; 30:84-99
Hussain F, Hojjati M, Okamoto M, Gorga RE. Polymer-matrix nanocomposites, processing, manufacturing, and application: an overview. Journal of Composite Materials. 2006; 40(17):1511-1575
Grunlan JC, Grigorian A, Hamilton CB, Mehrabi ARJ. Applied Polymer Science. 2004; 93:1102-1109
Huang Q, Yu H, Ru QJ. Food Science. 2010; 75:R50-R57
Theng KG. The Chemistry of Clay-Organic Reactions. London, UK: Adam Hilger; 1974
Nemecz E. Clay Minerals. Budapest, Hungary: Akademiai Kiado; 1981
Ogawa M, Kuroda K. Chemical Reviews. 1995; 95:399-438
Vaccari A. Catalysis Today. 1998; 41:53-71
Chung HE, Kim IS, Baek M, Yu J, Choi SJ. Long-term cytotoxicity potential of anionic nanoclays in human cells. Toxicology and Environmental Health Sciences. 2011; 3(2): 129-133
Sanchez CJ, Parras J, Carretero MI. The effect of maturation upon the mineralogical and physicochemical properties of illitic-smectitic clays for pelotherapy. Clay Minerals. 2002; 37(3):457-463
Veniale F, Barberis E, Carcangiu G, Morandi N, Setti M, Tamanini M, Tessier D. Applied Clay Science. 2004; 25:135-148
Gorchakov VN, Dragun GN, Kolmogorov YP, Smelova VA, Tikhonova LI, Tysjachnova YV. Nuclear Instruments and Methods in Physics Research Section A. 2001; 470:437-440
Burzlaff A, Brethauer S, Kasper C, Jackisch BO, Scheper T. Cytometry, Part A. 2004; 62:65-69
Peterson CL, Perry DL, Masood H, Lin H, White JL, Hem SL, Fritsch C, Haeusler F. Pharmaceutical Research. 1993; 10:998-1004
Baes CF, Mesmer RE. The Hydrolysis of Cations. Vol. 95-98. New York: A Wiley-Interscience Publication; 1976. pp. 112-122
Zümreoglu-Karan B, Ay A. Layered double hydroxides—multifunctional nanomaterials. Chemical Papers. 2012; 66(1):1-10.
Choi SJ, Choy JH. Nanomedicine. 2011; 6:803-814
Oh, Jae-Min, et al. Cellular uptake mechanism of an inorganic nanovehicle and its drug conjugates: enhanced efficacy due to clathrin-mediated endocytosis. Bioconjugate Chemistry. 2006; 17(6):1411-1417
Ferencz Z. Mechanochemical Preparation and Structural Characterization of Layered Double Hydroxides and their Amino Acid-Intercalated Derivatives (Doctoral dissertation, szte; 2016
Desigaux L, Belkacem MB, Richard P, Cellier J, Leone P, Cario L, Leroux F, Taviot-Gueho C, Pitard B. Nano Letters. 2006; 6:199-204
Choy JH, Kwak SY, Jeong YJ, Park JS. Angewandte Chemie: International Edition. 2000; 39:4042-4045
Wong Y, Cooper HM, Zhang K, Chen M, Bartlett P, Xu ZP. Journal of Colloid and Interface Science; 369:453-459
Choy JH, Jung JS, Oh JM, Park M, Jeong J, Kang YK, Han OJ. Biomaterials. 2004; 25:3059-3064
Choi SJ, Oh JM, Choy JHJ. Physics and Chemistry of Solids. 2008; 69:1528-1532
Rahman MB, Basri M, Hussein MZ, Rahman RN, Zainol DH, Salleh AB. Applied Biochemistry and Biotechnology. 2004; 118:313-320
Jin S, Fallgren PH, Morris JM, Chen Q. Science and Technology of Advanced Materials. 2007; 8:67-70
Oh JM, Park M, Kim ST, Jung JY, Kang YK, Choy JHJ. Physics and Chemistry of Solids. 2006; 67:1024-1027
Kim JY, Choi SJ, Oh JM, Park T, Choy JHJ. Nanoscience and Nanotechnology. 2007; 7:3700-3705
Oh JM, Choi SJ, Lee GE, Han SH, Choy JH. Advanced Functional Materials. 2009; 19:1-8
Carretero MI, Pozo M. Clay and non-clay minerals in the pharmaceutical industry: Part I. Excipients and medical applications. Applied Clay Science. 2009; 46(1):73-80
Bolger R. Industrial Minerals. 1995 August:52-63
Ferrand T, Yvon J. Applied Clay Science. 1991; 6:21-38
Poensin D, Carpentier PH, Féchoz C, Gasparini S. Effects of mud pack treatment on skin microcirculation. Joint Bone Spine. 2003; 70(5):367-370
Summa V, Tateo F. Applied Clay Science. 1998; 12:403-417
Cara S, Carcangiu G, Padalino G, Palomba M, Tamanini M. Applied Clay Science. 2000; 16:125-132
Gupta G, Gardner WJ. Hazardous Materials. 2005; 118:81-83
Wang X, Du Y, Luo J. Biopolymer/montmorillonite nanocomposite: preparation, drug-controlled release property and cytotoxicity. Nanotechnology. 2008; 19(6):065707
Tarnawski A, Pai R, Itani R, Wyle FA. Digestion. 1999; 60:449-455
Doborozsi D. Oral liquid mucoadhesive compositions. U.S. Patent 6.638.521; 2003
Kim TH, Lee JA, Choi SJ, Oh JM. Polymer coated CaAl-layered double hydroxide nanomaterials for potential calcium supplement. International Journal of Molecular Sciences. 2014; 15(12):22563-22579
Al-Beitawi NA, Momani Shaker M, El-Shuraydeh KN, Bláha J. Effect of nanoclay minerals on growth performance, internal organs and blood biochemistry of broiler chickens compared to vaccines and antibiotics. Journal of Applied Animal Research. 2017; 45(1):543-549
Desai MP, Labhasetwar V, Waltwr E, Levy RJ, Amidon GL. The mechanism of uptake of biodegradable microparticles in Caco-2 cells in size dependent. Pharmaceutical Research. 1997; 14:1568-1573
Weiss J, Takhistov P, McClements J. Functional material in food nanotechnology. Journal of Food Science. 2006; 71(9):107-116
Ramirez-Mella M, Hernandez-Mendo O. Nanotechnology in animal production. Tropical and Subtropical Agroecosystems. 2010; 12(3):423-429
Sawors F, Pineda L, Hotowy A, Jaworski S, Prasek M, Sawors E. Nanonutrition of chicken embryos. The effects of silver nanoparticles and ATP on expression chosen genes involved in myogenesis. Archives of Animal Nutrition. 2013; 67(5):347-355
Ghithrani BD, Chan WC. Elucidating the mechanism of cellular uptake and removal of protein-coated gold nanoparticles of different sizes and shapes. Nano Letters. 2007; 7:1542-1550
Verma NK, Moore E, Blau W, Volkov Y, Ramesh Babu P. Cytotoxicity evaluation of nanoclays in human epithelial cell line A549 using high content screening and real-time impedance analysis. 2012
Floody MC, Theng BKG, Reyes P, Mora ML. Natural nanoclays: Applications and future trends: A Chilean perspective. Clay Minerals. 2009; 44:161-176
Suresh R, Borkar SN, Sawant VA, Shende VS, Dimble SK. Nanoclay drug delivery system. International Journal of Pharmaceutical Sciences and Nanotechnology. 2010; 3:901-905
Dong Y, Feng SS. Poly(D,L-lactide-co-glycolide)/montmorillonite nanoparticles for oral delivery of anticancer drugs. Biomaterials. 2005; 26:6068-6076
Lin FH, Lee YH, Jian CH, Wong JM, Shieh MJ, Wang CY. A study of purified montmorillonite intercalated with 5-fluorouracil as drug carrier. Biomaterials. 2002; 23:1981-1987
Nayak PL, Sahoo D. Chitosan-alginate composites blended with cloisite 30B as a novel drug delivery system for anticancer drug paclitaxel. International Journal of Plastics Technology. 2011; 15:68-81
Forni F, Iannuccelli V, Coppi G, Bernabei MT. Effect of montmorillonite on drug release from polymeric matrices. Archiv der Pharmazie (Weinheim). 1989; 322(11):789-793
Lee W-F, Fu Y-T. Effect of montmorillonite on the swelling behavior and drug-release behavior of nanocomposite hydrogels. Journal of Applied Polymer Science. 2003; 89(13):3652-3660
Lin F-H, Chen C-H, Cheng WTK, Kuo T-F. Modified montmorillonite as vector for gene delivery. Biomaterials. 2006; 27(17):3333-3338
Viseras C, Aguzzi C, Cerezo P, Lopez-Galindo A. Uses of clay minerals in semisolid health care and therapeutic products. Applied Clay Science. 2007; 36(1-3):37-50
Takahashi T, Yamada Y, Kataoka K, Nagasaki Y. Preparation of a novel PEG-clay hybrid as a DDS material: Dispersion stability and sustained release profiles. Journal of Controlled Release. 2005; 107(3):408-416
des Rieux A, Fievez V, Garinot M, Schneider Y-J, Préat V. Nanoparticles as potential oral delivery systems of proteins and vaccines: A mechanistic approach. Journal of Controlled Release. 2006; 116(1):1-27
Sun B, Ranganathan B, Feng S-S. Multifunctional poly_D,L-lactide-co-glycolide/montmorillonite_PLGA/MMT_ nanoparticles decorated by trastuzumab for targeted chemotherapy of breast cancer. Biomaterials. 2008; 29(4):475-486
Wang X, Du Y, Luo J. Biopolymer/montmorillonite nanocomposite: Preparation, drug-controlled release property and cytotoxicity. Nanotechnology. 2008; 19(6):065707
Depan D, Kumar AP, Singh RP. Cell proliferation and controlled drug release studies of nanohybrids based on chitosan-G-lactic acid and montmorillonite. Acta Biomaterialia. 2009; 5(1):93-100
Carretero MI. Clay minerals and their beneficial effects upon human health: A review. Applied Clay Science. 2002; 21(3-4):155-163
Marras SI, Kladi KP, Tsivintzelis I, Zuburtikudis I, Panayiotou C. Biodegradable polymer nanocomposites: The role of nanoclays on the thermomechanical characteristics and the electrospun fibrous structure. Acta Biomaterialia. 2008; 4(3):756-765
Zheng JP, Wang CZ, Wang XX, Wang HY, Zhuang H, Yao KD. Preparation of biomimetic three-dimensional gelatin/montmorillonite-chitosan scaffold for tissue engineering. Reactive and Functional Polymers. 2007; 67(9):780-788
Ambre AH, Katti KS, Katti DR. Nanoclay based composite scaffolds for bone tissue engineering applications. Journal of Nanotechnology in Engineering and Medicine. 2010; 1(3):031013
Joshi GV, Kevadiya BD, Patel HA, Bajaj HC, Jasra RV. Montmorillonite as a drug delivery system: Intercalation and in vitro release of timolol maleate. International Journal of Pharmaceutics. 2009; 374:53-57
Joshi GV, Patel HA, Kevadiya BD, Bajaj HC. Montmorillonite intercalated with vitamin B1 as drug carrier. Applied Clay Science. 2009; 45:248-253
Joshi GV, Kevadiya BD, Bajaj HC. Design and evaluation of controlled drug delivery system of buspirone using inorganic layered clay mineral. Microporous and Mesoporous Materials. 2010; 132:526-530
Joshi GV, Kevadiya BD, Mody HM, Bajaj HC. Confinement and controlled release of quinine on chitosan–montmorillonite bionanocomposites. Journal of Polymer Science Part B: Polymer Physics. 2012; 50:423-430
Joshi GV, Pawar RR, Kevadiya BD, Bajaj HC. Mesoporous synthetic hectorites: A versatile layered host with drug delivery application. Microporous and Mesoporous Materials. 2011; 142:542-548
Kevadiya BD, Joshi GV, Bajaj HC. Layered bionanocomposites as carrier for procainamide. International Journal of Pharmaceutics. 2010; 388:280-286
Kevadiya BD, Joshi GV, Mody HM, Bajaj HC. Biopolymer-clay hydrogel composites as drug carrier: Host–guest intercalation and in vitro release study of lidocaine hydrochloride. Applied Clay Science. 2011; 52:364-367
Kevadiya BD, Patel TA, Jhala DD, Thumbar RP, Brahmbhatt H, et al. Layered inorganic nanocomposites: A promising carrier for 5-fluorouracil (5-FU). European Journal of Pharmaceutics and Biopharmaceutics. 2012; 81:91-101
Kevadiya BD, Thumbar RP, Rajput MM, Rajkumar S, et al. Montmorillonite/poly-(ε-caprolactone) composites as versatile layered material: Reservoirs for anticancer drug and controlled release property. European Journal of Pharmaceutical Sciences. 2012; 47:265-272
Giannelis EP. Review: Polymer layered silicate nanocomposites. Advanced Materials. 1996; 8:29-35
Choy JH, Choi SJ, Oh JM, Park T. Clay minerals and layered double hydroxides for novel biological applications. Applied Clay Science. 2007; 36:122-132
Komine H. Simplified evaluation for swelling characteristics of bentonites. Engineering Geology. 2004; 71:256-279
Fudala AA, Palinko II, Kiricsi I. Preparation and characterization of hybrid organicinorganic composite materials using the amphoteric property of amino acids: Amino acid intercalated layered double hydroxide and montmorillonite. Inorganic Chemistry. 1999; 38:4653-4658
Zheng JP, Luan L, Wang HY, Xi LF, Yao KD. Study on ibuprefen/montmorillonite intercalation composites as drug release system. Applied Clay Science. 2007; 36:297-301
Kollar T, Palinko I, Konya Z, Kiricsi I. Intercalating amino acid guests into montmorillonite host. Journal of Molecular Structure. 2003; 651-653:335-340
Park JK, Choy YB, Oh JM, Kim JY, Hwang SJ, Choy JH. Controlled release of donepezil intercalated in smectite clays. International Journal of Pharmaceutics. 2008; 359:198-204
Park M, Kim CY, Lee DH, Choi CL, Choi J, Lee SR, Choy JH. Intercalation of magnesium-urea complex into swelling clay. Journal of Physics and Chemistry of Solids. 2004; 65:409-412
Baek M, Choy JH, Choi SJ. Montmorillonite intercalated with glutathione for antioxidant delivery: Synthesis, characterization, and bioavailability evaluation. International Journal of Pharmaceutics. 2012; 425:29-34
Gamiz E, Linares J, Delgado R. Assessment of two Spanish bentonites for pharmaceutical uses. Applied Clay Science. 1992; 6:359-368
Bolger R. Industrial minerals in pharmaceuticals. Industrial Minerals. 1995; 8:52-63
Sun B, Ranganathan B, Feng SS. Multifunctional poly(D,L-lactide-coglycolide)/montmorillonite (PLGA/MMT) nanoparticles decorated by trastuzumab for targeted chemotherapy of breast cancer. Biomaterials. 2008; 29:475-486
Cornejo J, Hermosin MC, White JL, Barnes JR, Hem SL. Role of ferric iron in the oxidation of hydrocortisone by sepiolite and palygorskite. Clays and Clay Minerals. 1983; 31:109-112
Ferrand T, Yvon J. Thermal properties of clay pastes for pelotherapy. Applied Clay Science. 1991; 6:21-38
Poensin D, Carpentier PH, Fechoz C, Gasparini S. Effects of mud pack treatment on skin microcirculation. Joint, Bone, Spine. 2003; 70:367-370
Sposito G, Skipper NT, Sutton R, Park SH, Soper AK, Greathouse JA. Colloquium paper: Surface geochemistry of the clay minerals. Proceedings of the National Academy of Sciences of the United States of America. 1999; 96:3358-3364
Aguzzi C, Cerezo P, Viseras C, Caramella C. Use of clays as drug delivery systems: Possibilities and limitations. Applied Clay Science. 2007; 36:22-36
Carretero MI, Pozo M. Clay and non-clay minerals in the pharmaceutical industry. Part I. Excipients and medical applications. Applied Clay Science. 2009; 46:73-80
Wang X, Du Y, Luo J. Biopolymer/montmorillonite nanocomposite: Preparation, drugcontrolled release property and cytotoxicity. Nanotechnology. 2008; 19:065707 (7pp). DOI: 10.1088/0957-4484/19/6/065707
Takahashi T, Yamada Y, Kataoka K, Nagasaki Y. Preparation of a novel PEG–clay hybrid as a DDS material: Dispersion stability and sustained release profiles. Journal of Controlled Release. 2005; 107:408
Vaiana CA, Leonard MK, Drummy LF, Singh KM, Bubulya A, Vaia RA, Naik RR, Kadakia MP. Epidermal growth factor: Layered silicate nanocomposites for tissue regeneration. Biomacromolecules. 2011; 12:3139-3146
Kevadiya BD, Bajaj HC. The layered silicate, montmorillonite (MMT) as a drug delivery carrier. 2013
Cypes SH, Saltzman WM, Giannelis EP. Organosilicate-polymer drug delivery systems: Controlled release and enhanced mechanical properties. Journal of Controlled Release. 2003; 90:163-169
Shameli K, Ahmad MB, Yunus WMZW, Rustaiyan A, Ibrahim NA, Zargar M, Abdollahi Y. Green synthesis of silver/montmorillonite/chitosan bionanocomposites using the UV irradiation method and evaluation of antibacterial activity. International Journal of Nanomedicine. 2010; 5:875-887
Browne JE, Feldkamp JR, White JL, Hem SL. Characterisation and adsorptive properties of pharmaceutical grade clays. Journal of Pharmaceutical Sciences. 1980; 69:816-823
Lagaly G. Pesticide-clay interactions and formulations. Applied Clay Science. 2001; 18:205-209
Tolls J. Sorption of veterinary pharmaceuticals in soils: A review. Environmental Science & Technology. 2001; 35:3397-3406
Yano K, Usuki A, Okada A. Synthesis and properties of polyimide-clay hybrid films. Journal of Polymer Science Part A: Polymer Chemistry. 2000; 35:2289-2294
Zhang Y, Long M, Huang P, Yang H, Chang S, Hu Y, Tang A, Mao L. Intercalated 2D nanoclay for emerging drug delivery in cancer therapy. 2016
Brigatti MF, Galan E, Theng BKG. Structure and mineralogy of clay minerals. Developments in Clay Science. 2013; 5:21-81
Brown G, Brindley GW. Crystal structures of clay minerals and their Xray identification. Journal of Minerals Society. 1980;305-356. DOI: 10.1016/j.jenvman.2011.05.031
Dawson JI, Oreffo ROC. Clay: New opportunities for tissue regeneration and biomaterial design. Advanced Materials. 2013; 25:4069-4086
Mousa M, Evans ND, Oreffo ROC, Dawson JI. Clay nanoparticles for regenerative medicine and biomaterial design: A review of clay bioactivity. Biomaterials. 2018; 159:204-214
Kryuchkova M, Danilushkina A, Lvo Y, Fakhrullin R. Evaluation of toxicity of nanoclays and graphene oxide in vivo: A Paramecium caudatumstudy. Environmental Science: Nano. 2016; 3:442
Lvov YM, DeVilliers MM, Fakhrullin RF. The application of halloysite tubule nanoclay in drug delivery. Expert Opinion on Drug Delivery. 2016; 13:977-986
Neumann BS, Sansom KG. The rheological properties of dispersions of laponite, a synthetic hectorite-like clay, in electrolyte solutions. Clay Minerals. 1971; 9:231-243
Olphen EHV. Data Handbook for Clay Materials and Other Nonmetallic Minerals. 1979
Drever JI. The Geochemistry of Natural Waters. Englewood Cliffs, NJ: Prentice-Hall, Inc. 1982
Ruzicka B, Zaccarelli E. A fresh look at the Laponite phase diagram. Soft Matter. 2011; 7:1268
Galan E. Properties and applications of palygorskite-sepiolite clays. Clay Minerals. 1996; 31:443-453
Jones BF, Galan E. Sepiolite and palygorskite. Reviews in Mineralogy and Geochemistry. 1988; 19(1):631-674
Lvov YM, Shchukin DG, Mohwald H, Price RR. Halloysite clay nanotubes for controlled release of protective agents. ACS Nano. 2008; 2:814-820
Li PR et al. Evaluation on cytotoxicity and genotoxicity of the exfoliated silicate nanoclay. ACS Applied Materials & Interfaces. 2010; 2:1608-1613
Castro-Smirnov FA et al. Cellular uptake pathways of sepiolite nanofibers and DNA transfection improvement. Scientific Reports. 2017; 7:5586
Rawat K, Agarwal S, Tyagi A, Verma AK, Bohidar HB. Aspect ratio dependent cytotoxicity and antimicrobial properties of nanoclay. Applied Biochemistry and Biotechnology. 2014; 174:936-944